polyhedral oligomeric silsesquioxane (poss) suppresses 3068 dx.doi.org/10.1021/bm2006938 |...
Post on 20-Apr-2020
Embed Size (px)
Published: June 15, 2011
r 2011 American Chemical Society 3066 dx.doi.org/10.1021/bm2006938 | Biomacromolecules 2011, 12, 3066–3077
Polyhedral Oligomeric Silsesquioxane (POSS) Suppresses Enzymatic Degradation of PCL-Based Polyurethanes Xinzhu Gu,† Jian Wu,† and Patrick T. Mather*
Syracuse Biomaterials Institute, Department of Biomedical and Chemical Engineering, Syracuse University, Syracuse, New York 13244, United States
bS Supporting Information
Biostability is of critical importance for biomaterials applied for long-term medical implants and the biostability of polymeric biomaterials is of paramount importance for many applications. Thermoplastic polyurethanes (TPUs), multiblock copolymers composed of hard and soft segments, have figured prominently in the field of medical plastics for reasons discussed below. In TPUs, the hard segment block consists of a diisocyanate and a chain extender, whereas the soft segment is usually a polyol, either hydroxyl- or amine- terminated polyester, polyether, or polycar- bonate. The flexible soft segment gives the TPUs great elasticity, whereas the hard segment contributes strength. Generally speak- ing, the two segments are incompatible with each other and tend to form a nanoscale phase-separated morphology. Because of their great potential in tailoring polymer structures, polyurethanes have unique mechanical properties and good biocompatibility that make them ideal for many implantable biomedical devices, including artificial heart components, heart valves, vascular grafts, and mam- mary prostheses.1�3 The use of polyurethanes for biomedical implants was first suggested by Boretos and Pierce in 1967.4 Since their introduction, many different polyurethanes have been evaluated for their stability in the biological environment using both in vitro and in vivo test procedures.5�7 Nevertheless, it has been recognized that polyester-based polyurethanes are not suitable for long-term implant because of their susceptibility to hydrolytic degradation. Polyether- based polyurethanes, while hydrolytically stable, are subject to oxidative degradation.
Both poly(ε-caprolactone) (PCL) and poly(ethylene glycol) (PEG) polymers selected for incorporation within TPUs of the
present study are biocompatible and nonimmunogenic. So far, there have been several PCL- or PEG-based biomedical products for various clinical uses approved by the U.S. Food and Drug Administration (FDA).8,9 PCL is one of the most promising synthetic polymers that can degrade in contact with microor- ganisms.10�12 The related enzymatic hydrolytic degradation of PCL-based polymers has also been investigated, especially in the presence of ester-bond cleavage enzymes.13�17 Lipases are one of the most popularly studied enzymes to catalyze the cleavage of ester bonds by transesterification,18 although they do not occur naturally in the humanbody. Importantly, semicrystalline PCLblocks make the associated polyurethanes stiff and hydrophobic, limiting their compatibility with soft tissues and the range of potential applications. This problem might be overcome for water-contacting applications by introducing hydrophilic blocks such as poly(ethylene glycol),19,20 the approach adopted in our present work.
Poly(ethylene glycol) (PEG) is one of themost widely studied synthetic polymers used for designing hydrogels of use in the biomedical applications. The intrinsic hydrophilicity of PEG- based hydrogels repels nonspecific protein adsorption and resists bacterial and animal cell adhesion.21�23 Their elastic and soft nature imparts to the TPUs low mechanical and frictional irritation when in contact with tissues and organs. However, PEG-based polyurethanes have generally exhibited poor me- chanical properties.20 The properties of these polymers can be
Received: May 20, 2011 Revised: June 14, 2011
ABSTRACT: In this Article, we studied the enzymatic hydrolytic biodegradation behavior of a novel multiblock thermoplastic polyurethane (TPU) system, which incorporates polyhedral oli- gomeric silsesquioxane (POSS) into linear biodegradable thermo- plastic polyurethanes containing poly(ε-caproactone) (PCL) and polyethylene glycol (PEG) blocks. The biodegradation behavior of POSS-PCL-PEG TPUs was characterized by proton nuclear magnetic resonance spectroscopy (1H NMR), differential scan- ning calorimetry (DSC), tensile tests, scanning electron microscopy (SEM), and wavelength dispersive X-ray spectrometry (WDS) after enduring 22-day accelerated enzymatic hydrolytic degradation tests. POSS incorporation significantly suppressed in vitro enzymatic hydrolytic degradation of PCL-PEG-based multiblock TPUs by a surface passivation mechanism. WDS observations revealed that the covalently bonded POSS moieties developed a near-continuous and robust POSS-layer after initial degradation, which prevented ester bonds of PCL from enzymatic attack, thereby inhibiting further degradation. These striking results provide a new strategy to fabricate the polyester-based biostable thermoplastic polyurethanes (TPUs) of potential use in long-term surgical implants.
3067 dx.doi.org/10.1021/bm2006938 |Biomacromolecules 2011, 12, 3066–3077
improved by either blending24 or copolymerization.19,25�29 Because of the combination of great advantages of PCL andPEG, PCL-PEG- based copolymers might have great potential application in biome- dical fields including drug delivery, cell encapsulation, and tissue engineering.26,28,30,31 Indeed, Skarja and Woodhouse have devel- oped a family of biodegradable segmented polyurethanes, which has potential for use in soft tissue engineering applications.32�34The hard segments of these materials are composed of a phenylalanine-based diester chain extender and lysine diisocyanate, whereas the soft segments are either a PEG or PCL diol. It was found that the degradation rate and mechanical properties of these materi- als could be optimized by blending the PCL-based and PEG- based polyurethanes.24 Because of its vulnerability to hydro- lytic and oxidative degradation, PCL-PEG-based copolymers have proven to be unsuitable for long-term implantation. In this manuscript, we attempted to overcome this limitation through incorporation of a biostable moiety, POSS, which we now describe.
Polyhedral oligosilsesquioxane (POSS) is a class of hybrid molecules with an inorganic silicon�oxygen cage (Si8O12) and eight variable organic side groups pendant to each silicon vertex of the cage with the size of 1�3 nm. The silica-like framework renders POSS cages chemically stable, nontoxic, and mechani- cally robust.35,36 Our past work on POSS polyurethanes con- cerned microstructure-deformation studies,37,38 biodegradation,39
controlled drug delivery,40 biocompatibility,41 and hydrogel for- mation.42 Kannan et al. conducted in vitro hydrolysis and oxidation tests to assess the degradative resistance of polyhedral oligosilses- quioxane integrated poly(carbonate-urea) urethane (POSS-PCU).43
Their studies revealed that all samples showed no significant difference in their compliance and elasticity after a 70 day hydrolysis and oxidation test, indicating striking biostability. The authors proposed that POSS nanocores covalently incorporated in PCU chains impart a type of “protective” or “shielding effect” on the soft phase, thereby preserving its elasticity and compliant properties in oxidation and hydrolysis. Polycarbonate-urethane itself, however, possesses a greater biostability than does polyether-urethane and polyester-urethane.35,44�46 How to change the more common polyether- and polyester-based urethanes from a biodegradable form to a biostable form by incorporation of POSS (or other means) has not yet been reported.
Here we report on a series of new PCL- and PEG-based multiblock thermoplastic polyurethanes (TPUs) incorporating polyhedral oligosilsesquioxane (POSS). In this system, the POSS moieties, when covalently incorporated with PEG and PCL macromers, can be expected to aggregate and crystallize to form nanoscale crystals42,47 induced by microphase separation due to thermodynamic incompatibility among hydrophilic PEG and hydrophobic POSS and PCL. Consequently, these crystallized moieties can become the physical cross-links of a unique hybrid hydrogel in the water-swollen state. For comparison, we also synthesized PCL-PEG TPUs without POSS, revealing the influ- ence of POSS moieties on the enzymatic hydrolytic degradation behaviors of PCL-PEG-based TPUs in lipase solution.Moreover, we compared the influence of POSS incorporation strategies, particularly physical blending versus covalent bonding on the enzymatic degradation behaviors of TPUs.
Sample Preparation. Multiblock thermoplastic polyurethanes (TPUs) were synthesized from polycaprolactone (PCL)-diol, polyethylene
glycol (PEG), 2,2,4-trimethyl-1,3-pentane (TMP) POSS diol (R-group = iBu), hereafter “POSS diol” (99.5%, Hybrid Plastics), and lysine methyl-ester diisocyanate (LDI) using a one-step technique, as shown in Scheme 1. First, PEG (1 kg/mol and 10 kg/mol, Fluka) was purified by preparing a THF solution, precipitating into n-hexane several times and then filtering. These steps were repeated several times. The purified powder was then dried in a vacuum oven at room temperature overnight. LDI (Kyowa Hakko Chemical) was purified by vacuum distillation at an oil bath temperature of 180 �C. PCL-diol (1.25 kg/mol, Sigma-Aldrich) and POSS diol were used without further purification. As a representative example, we describe the detailed procedure to prepare [PEG1k]50-[PCL1k]30-[POSS]20 from PEG 1 kg/mol, PCL1.25 kg/mol, and POSS diol. In a 100 mL thre